Theory of Electro-Optical Properties of Graphene Nanoribbons Kondayya Gundra1, ∗ and Alok Shukla1

arXiv:1008.3538v2 [cond-mat.mtrl-sci] 6 Jan 2011

1

Department of Physics, Indian Institute of Technology, Bombay, Mumbai 400076 INDIA

We present calculations of the optical absorption and electro-absorption spectra of graphene nanoribbons (GNRs) using a π−electron approach, incorporating long-range Coulomb interactions within the Pariser-Parr-Pople (PPP) model Hamiltonian. The approach is carefully bench marked by computing quantities such as the band structure, electric-field driven half metallicity, and linear optical absorption spectra of GNRs of various types, and the results are in good agreement with those obtained using ab initio calculations. Our predictions on the linear absorption spectra for the transversely polarized photons provide a means to characterize GNRs by optical probes. We also compute the electro-absorption spectra of the zigzag GNRs, and argue that it can be used to determine, whether or not, they have a magnetic ground state, thereby allowing the edge magnetism to be probed through non-magnetic experiments. PACS numbers: 78.20.Bh, 78.67.Wj, 73.22.Pr , 78.40.Ri

I.

INTRODUCTION

Discovery of graphene1 has stimulated intense research in the field from the point-of-view of both fundamental physics, and promising applications2–4 . Of particular interest are recently synthesized5 quasi-onedimensional (1D) nanostructures of graphene called graphene nanoribbons (GNRs) which have technologically promising electronic and optical properties because of the confinement of electrons owing to the reduced dimensions. As a result, numerous theoretical studies of electronic, transport, and optical properties of GNRs of various type have been performed over the years6–16 . The structural anisotropy of GNRs must exhibit itself in an anisotropic optical response with respect to the photons polarized along the length of the ribbons (x polarized, or longitudinally polarized) as against those polarized perpendicular to it (y polarized or transversely polarized), with GNRs being in the xy-plane. Despite its obvious importance, anisotropy in the optical response of GNRs has not been studied in any of the reported optical absorption calculations, which concentrate only on the longitudinal component of the spectra12–16 . In this work we study this anisotropy in detail, and make predictions which can be tested in optical experiments on oriented samples of GNRs, and can serve as a means for their optical characterization. Electro-absorption (EA) spectroscopy, which consists of measuring optical absorption in the presence of a static external electric (E) field, has been used extensively to probe the electronic structure and optical properties of conjugated polymers and other materials17 . GNRs, being π-conjugated systems, will also be amenable to similar EA probes, and, therefore, we have calculated the EA spectrum of zigzag GNRs (ZGNRs) in this work. ZGNRs have been predicted to possess a magnetic ground state, with oppositely oriented spins localized on the opposite zigzag edges of the ribbons6,8 . Our calculated EA spectra of ZGNRs depends strongly on whether, or not, they exhibit edge magnetism, thereby, allowing its detection

by optical means. Most of the theoretical approaches used to study the electronic structure of GNRs are broadly based upon: (a) tight-binding method,6,7,9 (b) Dirac equation approach, derived using the linearity of the band structure in the region of interest,18 (c) ab initio DFT and GW based approaches,10,11,13,15 and (d) Hubbard model based approaches.19–22 But, it is obvious from the chemical-structure of graphene and GNRs that the electrons close to the chemical potential are itinerant πelectrons which determine their low-energy excitations. In π-electron systems such as various aromatic molecules and conjugated polymers, it is well-known that role of electron-electron (e-e) interactions cannot be ignored when describing their electronic properties.23 Therefore, it is inconceivable that the long-range e-e interactions will be insignificant in graphene and related structures. The effective π-electron approaches such as the Pariser-ParrPople (PPP) model Hamiltonian,24 which incorporate long-range e-e interaction, have been used with considerable success in describing the physics of π-conjugated molecules and polymers.23 Computationally speaking, PPP model has the advantage of including the long-range Coulomb interactions of π electrons within a minimal basis, thereby allowing calculations on such systems with limited computer resources, as compared to the ab initio approaches. Indeed, in our earlier works we have used the PPP model to extensively to study the electronic structure and optical properties of finite π-electron systems such as conjugated molecules and oligomers at various levels of theory.25 Therefore, in this work, we have decided to extend our PPP model based approach to study the physics of GNRs in the bulk limit. Because, to the best of our knowledge, this is the first application of the PPP model to the GNR physics, we have carefully bench marked it for quantities such as the band structure, electric-field driven half metallicity, and linear optical absorption spectra against the published ab initio works on GNRs, and the results are in very good agreement with each other. The remainder of this paper is organized as follows.

In the next section, we outline the theoretical aspects of our work. In section III, we present and discuss our results. Finally, in section IV we present our conclusions and discuss the directions for the future work. II.

THEORETICAL DETAILS

The PPP model Hamiltonian,24 with one π-electron per carbon atom (half-filled case), is given by X tij (c†iσ cjσ + c†jσ ciσ ) + H=− U

X i

i,j,σ

ni↑ ni↓ +

X

Vij (ni − 1)(nj − 1)

(1)

i

arXiv:1008.3538v2 [cond-mat.mtrl-sci] 6 Jan 2011

1

Department of Physics, Indian Institute of Technology, Bombay, Mumbai 400076 INDIA

We present calculations of the optical absorption and electro-absorption spectra of graphene nanoribbons (GNRs) using a π−electron approach, incorporating long-range Coulomb interactions within the Pariser-Parr-Pople (PPP) model Hamiltonian. The approach is carefully bench marked by computing quantities such as the band structure, electric-field driven half metallicity, and linear optical absorption spectra of GNRs of various types, and the results are in good agreement with those obtained using ab initio calculations. Our predictions on the linear absorption spectra for the transversely polarized photons provide a means to characterize GNRs by optical probes. We also compute the electro-absorption spectra of the zigzag GNRs, and argue that it can be used to determine, whether or not, they have a magnetic ground state, thereby allowing the edge magnetism to be probed through non-magnetic experiments. PACS numbers: 78.20.Bh, 78.67.Wj, 73.22.Pr , 78.40.Ri

I.

INTRODUCTION

Discovery of graphene1 has stimulated intense research in the field from the point-of-view of both fundamental physics, and promising applications2–4 . Of particular interest are recently synthesized5 quasi-onedimensional (1D) nanostructures of graphene called graphene nanoribbons (GNRs) which have technologically promising electronic and optical properties because of the confinement of electrons owing to the reduced dimensions. As a result, numerous theoretical studies of electronic, transport, and optical properties of GNRs of various type have been performed over the years6–16 . The structural anisotropy of GNRs must exhibit itself in an anisotropic optical response with respect to the photons polarized along the length of the ribbons (x polarized, or longitudinally polarized) as against those polarized perpendicular to it (y polarized or transversely polarized), with GNRs being in the xy-plane. Despite its obvious importance, anisotropy in the optical response of GNRs has not been studied in any of the reported optical absorption calculations, which concentrate only on the longitudinal component of the spectra12–16 . In this work we study this anisotropy in detail, and make predictions which can be tested in optical experiments on oriented samples of GNRs, and can serve as a means for their optical characterization. Electro-absorption (EA) spectroscopy, which consists of measuring optical absorption in the presence of a static external electric (E) field, has been used extensively to probe the electronic structure and optical properties of conjugated polymers and other materials17 . GNRs, being π-conjugated systems, will also be amenable to similar EA probes, and, therefore, we have calculated the EA spectrum of zigzag GNRs (ZGNRs) in this work. ZGNRs have been predicted to possess a magnetic ground state, with oppositely oriented spins localized on the opposite zigzag edges of the ribbons6,8 . Our calculated EA spectra of ZGNRs depends strongly on whether, or not, they exhibit edge magnetism, thereby, allowing its detection

by optical means. Most of the theoretical approaches used to study the electronic structure of GNRs are broadly based upon: (a) tight-binding method,6,7,9 (b) Dirac equation approach, derived using the linearity of the band structure in the region of interest,18 (c) ab initio DFT and GW based approaches,10,11,13,15 and (d) Hubbard model based approaches.19–22 But, it is obvious from the chemical-structure of graphene and GNRs that the electrons close to the chemical potential are itinerant πelectrons which determine their low-energy excitations. In π-electron systems such as various aromatic molecules and conjugated polymers, it is well-known that role of electron-electron (e-e) interactions cannot be ignored when describing their electronic properties.23 Therefore, it is inconceivable that the long-range e-e interactions will be insignificant in graphene and related structures. The effective π-electron approaches such as the Pariser-ParrPople (PPP) model Hamiltonian,24 which incorporate long-range e-e interaction, have been used with considerable success in describing the physics of π-conjugated molecules and polymers.23 Computationally speaking, PPP model has the advantage of including the long-range Coulomb interactions of π electrons within a minimal basis, thereby allowing calculations on such systems with limited computer resources, as compared to the ab initio approaches. Indeed, in our earlier works we have used the PPP model to extensively to study the electronic structure and optical properties of finite π-electron systems such as conjugated molecules and oligomers at various levels of theory.25 Therefore, in this work, we have decided to extend our PPP model based approach to study the physics of GNRs in the bulk limit. Because, to the best of our knowledge, this is the first application of the PPP model to the GNR physics, we have carefully bench marked it for quantities such as the band structure, electric-field driven half metallicity, and linear optical absorption spectra against the published ab initio works on GNRs, and the results are in very good agreement with each other. The remainder of this paper is organized as follows.

In the next section, we outline the theoretical aspects of our work. In section III, we present and discuss our results. Finally, in section IV we present our conclusions and discuss the directions for the future work. II.

THEORETICAL DETAILS

The PPP model Hamiltonian,24 with one π-electron per carbon atom (half-filled case), is given by X tij (c†iσ cjσ + c†jσ ciσ ) + H=− U

X i

i,j,σ

ni↑ ni↓ +

X

Vij (ni − 1)(nj − 1)

(1)

i